synthesis, characterization and swelling behaviour ... synthesis, characterization and swelling...
Post on 03-May-2020
Embed Size (px)
_____________________________________________________________________________________________________ *Corresponding author: E-mail: firstname.lastname@example.org;
Asian Journal of Chemical Sciences 2(1): 1-13, 2017; Article no.AJOCS.32155
SCIENCEDOMAIN international www.sciencedomain.org
Synthesis, Characterization and Swelling Behaviour of Guar Gum-g-poly (Methyl Methacrylate)
Kartika Rathore1* and Sangeeta Loonker1
1Applied and Environmental Chemistry Laboratory, Department of Chemistry, Jai Narain Vyas
University, Jodhpur – 342011, Rajasthan, India.
This work was carried out in collaboration between both authors. Both authors have equally contributed to work. The final manuscript has been read and approved by both authors.
Editor(s): (1) Georgiy B. Shul'pin, Semenov Institute of Chemical Physics, Russian Academy of Sciences, Moscow,
(1) Baki Hazer, Bülent Ecevit University, Turkey. (2) Alang Michael Bong, Catholic University of Cameroon, Bamenda, Cameroon.
Complete Peer review History: http://www.sciencedomain.org/review-history/18172
Received 10 th February 2017 Accepted 5 th March 2017
Published 11 th March 2017
ABSTRACT In this work, polymer nanocomposite was synthesized based on guar gum (GG) and methyl methacrylate (MMA) by free radical graft copolymerization reaction using boric acid as a cross linking agent and hydrogen peroxide as an initiator in complete aqueous solution to make it environmental friendly. The composite was synthesized to be used as superabsorbent for the purpose of water absorption. Fourier transform infrared (FTIR) analysis was carried out to confirm grafting of methyl methacrylate onto guar gum. The morphological study of composite was carried out by scanning electron microscopy (SEM). Thermal gravimetric analysis (TGA) confirms the stability of nanocomposite. The composite was characterized by X-ray diffraction (XRD) to study its crystalline nature. The water absorption capacity of superabsorbent was measured in distilled water by free swelling method as a function of percentage swelling and found to be 3000%. The effect of reaction parameters such as guar gum concentration, monomer concentration, initiator concentration, cross-linker concentration and temperature was investigated. The percentage swelling of superabsorbent composite was studied at various pH values between 2.0 and 13.0. The swelling behaviour of composite was also examined in saline solutions. Result shows that swelling
Original Research Article
Rathore and Loonker; AJOCS, 2(1): 1-13, 2017; Article no.AJOCS.32155
capacity is decreased by increasing the ionic strength of swelling medium. This behavior is because of charge screening effect for monovalent cations as well as ionic crosslinking for multivalent cations.
Keywords: Percentage swelling; copolymerization; grafting; SEM; TGA; saline; charge screening. 1. INTRODUCTION Superabsorbent polymers are moderately cross- linked hydrophilic network materials that can absorb and retain large quantities of aqueous fluids while preserving their shapes . Because of the unique characteristics they are extensively applied in various fields such as agriculture and horticulture [2,3], hygienic products as disposable diapers and feminine napkins , wastewater treatment [5,6,7], bio-medical area as antibacterial materials  and drug delivery [9,10]. However the traditional superabsorbents are mainly based on fully organic petroleum based polymers with relatively higher production cost and poor environmental friendly properties . Thus new types of cost-efficient and eco- friendly superabsorbents derived from naturally available raw materials have long been desired. The modification of natural polymers is a promising method for the preparation of new materials. Graft copolymerization of vinyl monomers onto natural polymers is an efficient approach to achieve these materials. Superabsorbing resins were first developed with a view to utilize in agricultural materials and are typed by the hydrolysed corn starch-g-poly (acrylonitrile), H-SPAN . Presently, natural
macromolecules such as starch [13,14], cellulose , chitosan [16,17], gelatin , alginate  etc and their derivatives have been used as polymer matrix for preparing superabsorbents and the resulting materials also exhibited ameliorative properties. GG is a hydrophilic, nonionic polysaccharide extracted from the endospermic seed of the plant Cyamopsis tetragonalobus. It consists of a linear backbone of - (1-4)-linked D-mannose units and is solubilised by the presence of randomly attached-(1-6) - linked galactose units as side chains. GG and its derivatives form valuable ingredients for foods, cosmetics and pharmaceuticals . GG has better reactivity and can be facilely modified by grafting vinyl monomers onto its backbone to derive new materials with improved structure and performance . The main functions of guar gum are as viscosifier, thickener, emulsifier, binding agent, stabilizer, gelling agent, natural fibre and flocculant . In this paper, we have tried to synthesize and characterize new superabsorbent nanocomposite based on guar gum and methyl methacrylate in complete aqueous solution. The structure of guar gum is shown in Fig. 1.
Fig. 1. Structure of guar gum
Rathore and Loonker; AJOCS, 2(1): 1-13, 2017; Article no.AJOCS.32155
Guar gum (GG, Shri Ram Gum Industries Basni, Jodhpur), Methyl methacrylate (MMA stabilised for synthesis, Merck), Boric acid (H3BO3, Qualigens Fine Chemicals), Acetone (Fischer Scientific, Qualigens), Hydrogen peroxide (H2O2, Emplura 30% w/v) and Ethanol (C2H5OH, Emsure) All of these are used without further purification.
2.2 Synthesis of Guar gum-g-PMMA Superabsorbent Nanocomposites
Guar gum (GG) 1.6 % (w/v) was added in 50 mL of distilled water in a round-bottomed flask equipped with stirrer and thermostated water bath. The above solution was stirred for one hour. The monomer MMA (6% v/v) was added in above guar gum slurry and mixture was stirred for half an hour. Then required volume of initiator hydrogen peroxide (1mL/10mL) was added to generate radicals. Further 1% aqueous solution of cross-linker (prepared by heating 0.1 g boric acid in 10 mL distilled water) added in the mixture. The reaction mixture was continuously stirred and heated to 60ºC for about 3 hours. After that it was precipitated using excess of acetone and kept overnight. Then it was washed several times with mixture of distilled water and ethanol (60:40) to remove homopolymer and unreacted mass. The grafted product was dried in oven at 80ºC. Finally, the dried resulting product was pulverized into powder.
2.3 Absorbency or Swelling Measurement Absorbency of superabsorbent composite is measured by the free swelling method and
calculated in terms of percentage swelling. A 0.1 g of dry sample was immersed in distilled water at room temperature for 24 h to reach swelling equilibrium. The swollen gel was taken out, dried between folds of filter paper (blotting) and weighed. After weighing the swollen samples, the equilibrium water absorbency of the superabsorbent was calculated using Eq. (1)
W2 - W1 (1) W1
% Swelling is the equilibrium water absorbency of sample which are the averages of three measurements. W1 and W2 are the weight of the dry sample and water swollen sample respectively.
3. RESULTS AND DISCUSSION 3.1 Synthesis and Characterization The superabsorbent nanocomposite was synthesized by graft copolymerization of methyl methacrylate onto guar gum in presence of a cross-linking agent boric acid and hydrogen peroxide was used as an initiator. The peroxide is decomposed under heating and produced hydroxide radicals that abstract hydrogen from -OH groups of the guar gum backbone. This peroxide-saccharide redox system thus results in active centers capable of initiating radical polymerization of MMA to give a graft copolymer. Since a cross-linking agent, boric acid is present in the system, the copolymer has a crosslinked structure. The composite was characterized by FTIR to confirm grafting of MMA onto guar gum.
Fig. 2. (a) Dry composite (b) Swollen composite
% Swelling = x 100
Scheme 1. General mechanism for hydrogen peroxide initiated graft copolymerization of MMA
onto guar gum in presence of boric acid
3.2 SEM Analysis Scanning electron microscopy was used for analyzing surface morphology of prepared composite. Fig. 3 shows SEM micrographs of guar gum and prepared superabsorbent composite at different magnification obtained by
Rathore and Loonker; AJOCS, 2(1): 1-13, 2017; Article no.
Scheme 1. General mechanism for hydrogen peroxide initiated graft copolymerization of MMA onto guar gum in presence of boric acid
microscopy was used for analyzing surface morphology of prepared
3 shows SEM micrographs